Upcoming SlideShare
×

Modern theory of magnetism in metals and alloys

997 views

Published on

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total views
997
On SlideShare
0
From Embeds
0
Number of Embeds
1
Actions
Shares
0
0
0
Likes
0
Embeds 0
No embeds

No notes for slide

Modern theory of magnetism in metals and alloys

1. 1. Chapter 1 Introduction to Magnetism Magnetic properties originate in the spin degrees of freedom of electrons and their associated motion in solids. We ﬁrst describe the microscopic magnetic moments of electrons, and the formation of atomic magnetic moments due to strong Coulomb interactions in an atom with unﬁlled shell. Atomic magnetic moments change their nature when the atoms form a solid. The key to understanding the behavior of mag- netic moments in solids is the degree of electron localization. We brieﬂy introduce the concept of the metal and the insulator (i.e., the Mott insulator). Electrons in the latter are localized on each atom, so that their magnetic properties are described by the atomic magnetic moments and the magnetic interactions between them. We present in this chapter only a minimal discussion on the magnetism in insulators. On the other hand, electrons move from site to site over the entire crystal in metals, so that the magnetic properties are connected to the whole degrees of freedom of correlated electrons. Needless to say, the main theme of this book is the magnetism of metals and alloys. In the last section, we elucidate various magnetic structures in solids to provide a basic knowledge on magnetism. 1.1 Magnetic Moments Magnetic moment M in the electromagnetics is deﬁned by the torque N on a magnet under the magnetic ﬁeld H as N ≡ M × H. (1.1) It originates in electrons in the magnet. According to the classical electromagnetics, the coil-type local current i(r) due to electron motion causes a magnetic moment. It is given in the CGS-Gauss unit as [1] ML = 1 2c r × i(r)d3 x. (1.2) Y. Kakehashi, Modern Theory of Magnetism in Metals and Alloys, Springer Series in Solid-State Sciences 175, DOI 10.1007/978-3-642-33401-6_1, © Springer-Verlag Berlin Heidelberg 2012 1
2. 2. 2 1 Introduction to Magnetism Here c is the speed of light. i(r) is the current density of electrons, given by i(r) = − i eviδ(r − ri) with vi being the velocity of the electron and −e the charge of the electron at ri. Substituting the expressions into (1.2), we obtain ML = − i e 2mec li. (1.3) Here me is the mass of an electron and li denotes the angular momentum of elec- tron i. Equation (1.3) indicates that an electron with angular momentum l generates a magnetic moment, ml = − e 2mec l. (1.4) This is called the orbital magnetic moment for an electron. According to the quantum mechanics, an electron has its own magnetic moment called the spin magnetic moment [2]. It is given by ms = −ge e 2mec s. (1.5) Here s is the spin angular momentum of an electron with spin s = 1/2. The constant ge = 2.0023 is referred as the g-value of electron. The deviation from 2 is caused by the interaction with electro-magnetic ﬁelds. The spin magnetic moment was found ﬁrst experimentally by Stern and Gerlach in 1922, and was established theoretically in 1928 by Dirac in his relativistic theory of electrons [3]. In the following we as- sume that ge = 2 for simplicity. As seen from (1.5), the spin of an electron leads to the magnetic moment μB = e 2mec = 0.9274 × 10−20 emu. (1.6) Here is the Planck constant divided by 2π. The magnetic moment μB denotes the Bohr magneton, and is often used as a unit of the magnetic moment in atomic scale. Equations (1.4) and (1.5) indicate that an electron has the following magnetic moment in the atomic scale. m = ml + ms = −(l + 2s)μB, (1.7) and the total magnetic moment is given by M = − i (li + 2si)μB . (1.8)
3. 3. 1.2 Basic Hamiltonian 3 Here the angular momenta l and s are measured in units of = 1. The li and si at the right-hand-side (r.h.s.) of the above equation should be regarded as quantum mechanical operators, and ∼ means a quantum mechanical expectation value. In the following, we omit the minus sign at the r.h.s. of (1.8) for convenience bearing in mind that the real magnetic moments are opposite in direction. It should be noted that the nuclei in the magnet also have magnetic moments because they have their own spins. The size of their magnetic moments is however characterized by the nuclear magneton μN, which is deﬁned by μN = e 2mpc . (1.9) Here mp denotes the mass of proton. The nuclear magneton μN is only 1/1800 of the Bohr magneton μB because μN/μB = me/mp. Therefore the magnetism in solids is dominated by the magnetic moments of electrons. In the following equations, we adopt a unit of μB = 1 for simplicity. 1.2 Basic Hamiltonian Magnetic moments and magnetic properties are governed by the Hamiltonian of the system. The basic Hamiltonian of electrons in solids is given as follows in the second quantization. H = ψ† (r) − 1 2 ∇2 + vN(r) ψ(r)dr + 1 2 ψ† (r)ψ† r 1 |r − r | ψ r ψ(r)dr dr + ψ† (r) 1 2 ∇vN(r) × (−i∇) · 1 2 σ ψ(r)dr − ψ† (r)(l + 2s)ψ(r)dr · H. (1.10) Here we have adopted the units me = 1, = 1, and e = 1 for simplicity. ψ(r) = (ψ↑(r),ψ↓(r)) is the electron ﬁeld operator. vN(r) is the one electron potential en- ergy due to nuclei, and is given by vN(r) = − i Zi/|r −Ri|. Zi is the atomic num- ber of the atom at position Ri. H denotes the magnetic ﬁeld, and σ = (σx,σy,σz) denote the Pauli spin matrices given by σx = 0 1 1 0 , σy = 0 −i i 0 , σz = 1 0 0 −1 . (1.11) The ﬁrst term in the Hamiltonian (1.10) consists of the kinetic energy and the attractive potential due to nuclei, and describes the independent motion of electrons.
4. 4. 4 1 Introduction to Magnetism The second term denotes the electron–electron interaction, the third term denotes the spin–orbit interaction, and the last term is the Zeeman interaction due to magnetic ﬁeld. Note that in the above expression we have omitted the diamagnetic term which is proportional to the square of the magnetic ﬁeld [2], because we do not consider the diamagnetism in this book. In solids, we may express the ﬁeld operators by means of a basis set of wave- functions {ϕi(r)} as follows. ψσ (r) = i aiσ ϕi(r). (1.12) Here ϕi(r) are orthonormal basis functions. The sufﬁx i stands for a set of the atomic position i (quantum number n) and orbital L (momentum k) when we adopt atomic orbitals (one-electron eigen functions in solids) as the basis functions. Using the orthonormal basis set, we can express the Hamiltonian (1.10) as fol- lows. H = ijσ εij a† iσ ajσ + 1 2 ijklσσ Vijkla† iσ a† jσ akσ alσ + HSO + HZeeman. (1.13) Here εij (Vijkl) are the matrix elements for the independent electron (the Coulomb interaction) part of the Hamiltonian (1.10). They are given by εij = dr ϕ∗ i (r) − 1 2 ∇2 + vN(r) ϕj (r), (1.14) Vijkl = dr dr ϕ∗ i (r)ϕ∗ j (r )ϕk(r )ϕl(r) |r − r | . (1.15) The third and last terms at the r.h.s. of (1.13) are the spin–orbit interaction term and the Zeeman term, respectively. HSO = iαjγ ζiαjγ a† iαajγ , (1.16) HZeeman = − iαjγ (l + 2s)iαjγ a† iαajγ · H. (1.17) Here the spin–orbit interaction matrix elements ζiαjγ are given by ζiαjγ = dr ϕ∗ i (r) 1 2 ∇v(r) × (−i∇) ϕj (r) · (s)αγ . (1.18) In molecules and solids, atomic orbitals are often useful as the basis functions. ϕ (atom) i (r) = φinl |r − Ri| Ylm(r − Ri). (1.19) Here φinl(|r −Ri|) is a radial wave function for an atom located at Ri, the subscripts n and l denote the principal quantum number and the azimuthal quantum number,
5. 5. 1.2 Basic Hamiltonian 5 respectively. Ylm(r − Ri) is the spherical harmonics located at atom Ri, and m denotes the magnetic quantum number. In the application to solids, it is convenient to make use of real functions {Plν} instead of complex basis functions {Ylm}. The former called the cubic harmonics are constructed by linear combinations of spherical harmonics. Deﬁning the orbital L = (l,ν), the atomic functions for solids are written as follows. ϕinL(r) = φinl |r − Ri| Plν(r − Ri). (1.20) The cubic harmonics are constructed to yield the irreducible representation for the cubic symmetry of the point group in crystal. The s (l = 0) function belonging to the A1g representation for the cubic point symmetry is a constant function. Pa1g (r) = Y00 = 1 √ 4π . (1.21) The p (l = 1) functions belonging to the T1u representation are deﬁned as follows. Pt1uα(r) = 1 √ 2 (−Y11 + Y1,−1) = 3 4π x r , (1.22) Pt1uβ(r) = i √ 2 (Y11 + Y1,−1) = 3 4π y r , (1.23) Pt1uγ (r) = Y10 = 3 4π z r . (1.24) The d (l = 2) orbitals form the Eg (dγ ) and T2g (dε) representations. The d functions belonging to the Eg representation are given by Pegu (r) = Y20 = 5 4π 1 2 3z2 − r2 r2 , (1.25) Pegv (r) = 1 √ 2 (Y22 + Y2,−2) = 5 4π √ 3 2 x2 − y2 r2 . (1.26) The remaining d (l = 2) functions belonging to the T2g representation are given by Pt2gξ (r) = i √ 2 (Y21 + Y2,−1) = 5 4π √ 3 yz r2 , (1.27) Pt2gη (r) = 1 √ 2 (−Y21 + Y2,−1) = 5 4π √ 3 zx r2 , (1.28) Pt2gζ (r) = i √ 2 (−Y22 + Y2,−2) = 5 4π √ 3 xy r2 . (1.29)
6. 6. 6 1 Introduction to Magnetism Fig. 1.1 Atomic orbitals from s to d symmetry. The sign of wave functions is shown by + and − in the ﬁgure The angular dependence of the cubic harmonics is shown in Fig. 1.1. The spatial distribution of the atomic wave functions governs the electron hoppings in solids, thus determining the electronic and magnetic properties of solids. 1.3 Formation of Atomic Moments The electronic structure and related properties of an atom may be understood by an independent-electron picture. The spin–orbit interaction in the Hamiltonian (1.13) is smaller than the Coulomb interaction in the ‘light’ elements such as the 3d transition metals. We ﬁrst neglect the former, and treat the latter by means of the following approximation. a† iσ a† jσ akσ alσ = a† iσ alσ a† jσ akσ + a† iσ alσ a† jσ akσ − a† iσ akσ a† jσ alσ − a† iσ akσ a† jσ alσ − a† iσ a† jσ akσ alσ . (1.30) Here the average is taken with respect to an independent particle system which will be chosen later. Note that the two particle operator has been decoupled so that (1.30) exactly holds true when we take the average. This is called the Hartree–Fock approximation. In the Hartree–Fock approximation, the Hamiltonian (1.13) is reduced to H = ijσ hijσ a† iσ ajσ − 1 2 ijklσσ (Vijkl − Vijlkδσσ ) a† iσ alσ a† jσ akσ . (1.31)
7. 7. 1.3 Formation of Atomic Moments 7 Here hijσ is given as follows. hijσ = ϕ† iσ (r) − 1 2 ∇2 + vN(r) + dr n(r ) |r − r | ϕjσ (r) − dr dr ϕ† iσ (r) ψ† σ (r )ψσ (r) |r − r | ϕjσ r . (1.32) The Hartree–Fock one-electron wave functions {ϕiσ (r)} are determined by solv- ing the following self-consistent equations. − 1 2 ∇2 + vN(r) + dr n(r ) |r − r | ϕiσ (r) − j njσ dr ϕ∗ jσ (r )ϕiσ (r ) |r − r | ϕjσ (r) = εiσ ϕiσ (r). (1.33) Here εiσ is the Hartree–Fock energy eigen value. When we apply the Hartree–Fock independent particle Hamiltonian in the average , njσ is given by the Fermi dis- tribution function f (εjσ ) and n(r) = jσ f (εjσ )ϕ∗ jσ (r)ϕjσ (r) denotes a charge density in the Hartree–Fock approximation. The third term at the l.h.s. of (1.33) gives the electrostatic potential due to electrons. The last term also originates in the Coulomb interaction, but the wave functions have been exchanged due to the anti-symmetric property of the Slater determinant. It is referred as the exchange po- tential. The Hartree–Fock wave function is the best Slater determinant at the ground state according to the variational principle [4]. Taking the Hartree–Fock wavefunctions as the basis functions, one can express the Hartree–Fock Hamiltonian (1.31) as follows. H = iσ εiσ niσ − 1 2 ijσσ (Vijji − Vijij δσσ ) niσ njσ . (1.34) Here Vijji (Vijij ) is known as the Coulomb integral (exchange integral). (Note that Vijkl should more precisely be Viσjσ kσ lσ .) The second term at the r.h.s. is to elim- inate the double counting of Coulomb interaction in the Hartree–Fock one-electron energy. The exchange potential in the Hartree–Fock equation (1.33) is nonlocal. Slater proposed an approximate local exchange potential, using the free-electron wave functions. It is given as follows [4]. vexσ (r) = −3 3 4π 1/3 nσ (r)1/3 , (1.35) where nσ (r) is the electron density with spin σ. The effective potential in the Hartree–Fock self-consistent equation is spherical in the atomic system when we apply the potential (1.35). We can express the atomic
8. 8. 8 1 Introduction to Magnetism wave function for an electron as ϕnlmσ (r) = φnlσ (r)Ylm(ˆr). (1.36) Here φnlσ (r) is the radial wave function, and Ylm(ˆr) is the spherical harmonics. n, l, and m denote the principal quantum number, the azimuthal quantum number, and the magnetic quantum number, respectively. Orbitals l = 0,1,2,3,... are called s, p, d, f, ..., respectively. The nl shells are therefore written as ns, np, nd, nf, etc. In each shell, there are 2l + 1 degenerate orbitals. With the use of the Hartree–Fock atomic orbitals, a many electron state of an atom is expressed in the form of the Slater determinant. The ground-state electronic structure of an atom is constructed according to the Pauli principle. For example, in the case of Ar, we have the ground state 1s22s22p63s23p6. Since the outermost electron shell of Ar is closed, the magnetic moment of Ar vanishes. For an atom with an unﬁlled shell, the magnetic moment may appear. Since the total number of electrons (N), the total spin (S), and the total orbital moment (L) of an atom commute with the Hamiltonian, the eigen function Ψ should be speciﬁed by the set (NLMSMs): Ψ (NLMSMs), where L (S) and M (Ms) denote the magnitude and z component of orbital moment L (spin S), respectively. The eigen energy, on the other hand, should depend only on N, L, and S because of the rotational symmetry: EA(NLS). The ground state of electrons in an atom should be obtained by minimizing the Coulomb energy. The Coulomb interaction of the Hamiltonian for the unﬁlled shell is written as follows according to (1.13). HCoulomb = ν Uννnν↑nν↓ + ν>ν Uνν − 1 2 Jνν nνnν − 2 ν>ν Jνν sν · sν . (1.37) Here ν denotes an orbital lm (m = −l ...l). nν (sν) denotes the charge (spin) density operator for electrons in the orbital ν. We have taken into account the Hartree–Fock Coulomb and exchange interactions, Uνν = Vνν ν ν and Jνν = Vνν νν , and omitted the other types of interactions. The ﬁrst term at the r.h.s. of (1.37) denotes the intra- orbital Coulomb interaction, the second term expresses the inter-orbital interaction, and the third term the exchange interaction between the spins on different orbitals. Note that Uνν > Uνν (ν = ν ) > Jνν > 0. Typical values of Coulomb interactions are Uνν ≈ 20 eV, Uνν − Uνν ≈ 2 eV, and Jνν ≈ 0.9 eV for 3d transition-metal elements [5]. Note that N stands for the total number of electrons in the unﬁlled shell when the Hamiltonian (1.37) is applied. The intra-orbital Coulomb interaction (i.e., the ﬁrst term at the r.h.s. of (1.37)) acts to reduce the doubly occupied states on the same orbital so that it creates active spins on the orbitals of an unﬁlled shell. The third term in (1.37) aligns the active spins on the orbitals because Jνν > 0. These effects suggest that the magnitude of the total spin S is maximized at the ground state. This is known as Hund’s ﬁrst rule, and therefore Jνν are often called the Hund-rule couplings. On the other hand, the
9. 9. 1.3 Formation of Atomic Moments 9 second term in (1.37) is the energy associated with the conﬁguration of electrons on different orbitals. One might expect that such an interaction energy is reduced when electrons move around the nucleus in the same direction avoiding each other. Thus we expect that the magnitude of the total angular momentum L should be maximized at the ground state under the maximum magnitude of total spin. This is referred as Hund’s second rule. The ﬁrst and second Hund rules are veriﬁed by the full Hartree–Fock numerical calculations. The maximum S and L at the ground state are obtained by using the Pauli principle and the Hund rule, especially from the conditions S = Ms(Max) and L = M(Max) under the maximum S that corresponds to the state Ψ (NLLSS): S = ⎧ ⎪⎨ ⎪⎩ N 2 for N ≤ 2l + 1, 4l + 2 − N 2 for N > 2l + 1, (1.38) L = 1 2 N(2l + 1 − N) for N ≤ 2l + 1, 1 2 (N − 2l − 1)(4l + 2 − N) for N > 2l + 1. (1.39) The ground state Ψ (NLMSMs) is (2L + 1)(2S + 1)-fold degenerate. The mul- tiplet is written as 2S+1LJ where L takes S, P, D, F, G, H,... according to L = 0,1,2,3,4,5,..., and J (= |L ± S|) is the total angular momentum. These properties are summarized in Fig. 1.2 for 3d transition metal atoms. The value of J at the ground state is determined by the spin–orbit interaction. The spin–orbit interaction (1.16) in the atomic system can be written as HSO = ναν γ ζnl (l)νν · (s)αγ a† ναaν γ . (1.40) Here ζnl = 1 2 ∞ 0 φnl(r) 2 dV dr r dr > 0. (1.41) Assume that the ground state is determined by the Hund rule, and the temperature is such that the corresponding thermal energy is much lower than that of the ﬁrst ex- cited state of the Coulomb interaction, i.e., the Hund-rule coupling JH: kBT JH. Here JH is an average value of {Jνν }, and kB denotes Boltzmann’s constant. More- over the spin–orbit interaction energy is much smaller than JH in 3d transition metals. In this case, we can neglect all the excited state of the Coulomb interac- tions, and limit the states to the (2L + 1)(2S + 1) dimensional Hund-rule subspace: {Ψ (NLMSMs)}. We can then verify the following relation in the subspace. Ψ (NLMSMs) HSO Ψ NLM SMs = λ(NLS) Ψ (NLMSMs) L · S Ψ NLM SMs . (1.42)
10. 10. 10 1 Introduction to Magnetism Fig. 1.2 The ground state of atoms with 3d unﬁlled shell. N and mz denote the d electron number and the orbital magnetic quantum number, respectively. Electron conﬁguration for each N in the upper row of the ﬁgure shows the state Ψ (NLLSS) leading to the total spin S and the orbital angular momentum L at the ground state. J denotes the total angular momentum. The ground state multiplets (GS) are expressed as 2S+1LJ . The experimental values of the spin–orbit coupling constant λ are given. Examples of the 3d transition metal ions are also given in the bottom row Thus we have an effective Hamiltonian for the spin–orbit interaction in the Hund- rule subspace as follows. HSO = λ(NLS)L · S. (1.43) The coefﬁcient λ(NLS) is obtained by comparing the diagonal matrix element of HSO for the state Ψ (NLLSS) obtained from (1.40) with that of the r.h.s. of (1.43). λ(NLS) = ⎧ ⎪⎨ ⎪⎩ ζnl N for N ≤ 2l + 1, − ζnl 4l + 2 − N for N > 2l + 1. (1.44) Because ζnl > 0, λ(NLS) > 0 for N ≤ 2l + 1 and λ(NLS) < 0 for N > 2l + 1. Thus, J = |L − S| is realized for N ≤ 2l + 1, and J = |L + S| for N > 2l + 1 at the ground state among possible states J = |L+S|,|L+S −1|,...,|L−S|. Therefore J = |L − S| is the ground-state in the light transition-metal elements and the light
11. 11. 1.4 Metal and Insulator in Solids 11 rare-earth elements, and J = |L + S| is the ground state in the heavy transition- metal elements and the heavy rare-earth elements. Note that the typical value of the spin–orbit coupling is only one tenth of the Hund rule coupling (JH ∼ 1 eV) in the case of 3d transition metal ions as shown in Fig. 1.2. When the spin–orbit coupling is signiﬁcant as in the rare-earth atoms, the ground-state should be (2J + 1)-fold degenerate instead of (2S + 1)(2L + 1) fold. Ions such as Ti2+, V3+, and Cr4+, for example, have two electrons in the d shell (see the N = 2 column in Fig. 1.2). The Hund rule tells us that the total spin and orbital angular momenta at the ground state are S = 1 and L = 3, respectively. Be- cause the spin–orbit coupling λ > 0 in the light atoms, the total angular momentum at the ground state is given by J = 3 − 1. Thus we have the ground-state multiplet 3F2 according to the notation 2S+1LJ . In the same way, the ion Co2+ has 7 elec- trons in the d shell. According to the Hund rule, we ﬁnd the ground-state spin and orbital momenta S = 3/2 and L = 3, respectively. Because the spin–orbit coupling λ < 0 in the heavy atoms, the total angular momentum is given by J = 9/2. Thus we obtain the ground-state multiplet 4F9/2 for Co2+ ion. When the external magnetic ﬁeld H is applied to the atoms, the energy due to the magnetic ﬁeld is given by −gJ μBJzH. Here gJ is Landé’s g factor and is given by gJ = 3/2 + [S(S + 1) − L(L + 1)]/2J(J + 1). The susceptibility which is deﬁned by the induced magnetization divided by H is then given by χ = g2 J μ2 BJ(J + 1) 3kBT . (1.45) The above temperature dependence is referred as the Curie law, and C ≡ g2 J μ2 BJ(J + 1)/3kB is called the Curie constant. The observation of the Curie law in the susceptibility measurement is regarded as an indication of the existence of local magnetic moments. 1.4 Metal and Insulator in Solids When atoms form a solid, electrons in the outermost shell of atoms start to hop from atom to atom via overlap between atomic orbitals. The question then is whether electrons tend to remain in each atom or to itinerate in the solid. In the case of the former, atomic magnetic moments are well deﬁned in solids and their properties are expected to be explained from the atomic point of view. In the case of the latter, magnetic properties may be quite different from those expected from atomic ones and one has to start from the itinerant limit in order to explain their magnetism. Whether electrons in solids are movable or not is governed by the detailed bal- ance between the energy gain due to electron hopping and the loss of Coulomb in- teraction. The simplest example may be the case of the hydrogen molecule H2. Ac- cording to the molecular orbital picture, the 1s atomic orbitals split into the bonding state with energy ε0 − |t| and the anti-bonding state with energy ε0 + |t| when hy- drogen atoms form a molecule. Here ε0 denotes the atomic ground state, and t is the
12. 12. 12 1 Introduction to Magnetism electron hopping integral which is deﬁned by atomic potential v(r) and wave func- tion ϕ(r) as t = ϕ(r − R)v(r − R)ϕ(r)dr. The bonding orbital is occupied by two electrons according to the Pauli principle. It leads to the total energy gain 2|t|. This is the covalent bond in the hydrogen molecule. In this state, electrons hop from one atom to another, and thus they are movable. The covalent bond is stabilized by the kinetic energy gain of independent electrons. It consists of the polarized state in which the 1s orbital of an atom is doubly occupied and the orbital of another atom is unoccupied, and the neutral state in which each atomic orbital is occupied by an electron. When the Coulomb interaction between electrons are taken into account, the covalent bonding state is not necessarily stable because it contains the polariza- tion state with double occupancy on an atomic orbital. Assume that the loss of the intraatomic Coulomb interaction energy in the covalent bonding state is given by U, and consider the neutral-atom state as the state in which each electron is localized on an atom. The total energy in the covalent bonding state is given by E(covalent) = 2ε0 − 2|t| + U, while the energy in the neutral atom state is given by E(neutral) = 2ε0. Thus, the neutral atom state is realized when the following condition is satisﬁed. 2|t| < U. (1.46) This condition is satisﬁed when the interatomic distance goes to inﬁnity because |t| goes to zero. Thus the neutral atom state in which electrons are localized on each atom and each atom has a well deﬁned local magnetic moment s = 1/2 is realized in the atomic limit. In solids, we expect the same behavior as found in the hydrogen molecule. Let us consider the behavior of electrons when atoms form a solid. Electrons in solids move in a potential obtained by a superposition of the atomic potentials i v(r − Ri). Here v(r − Ri) denotes the atomic potential on site i. When we adopt the atomic orbitals {ϕiν(r − Ri)} as the basis functions and assume the orthogonality between the orbitals, the Hamiltonian for electrons on the outermost shells in solids may be obtained from (1.13) as H = H0 + HCoulomb, (1.47) H0 = iν εiνniν + iνjν tiνjν a† iνσ ajν σ , (1.48) HCoulomb = iν Uiννniν↑niν↓ + i ν>ν Uiνν − 1 2 Jiνν niνniν − 2 i ν>ν Jiνν siν · siν . (1.49) Here εiν is the atomic level for the orbital ν of site i, and tiνjν the transfer integral between the orbital ν at site i and the orbital ν at site j. The latter is expressed in
13. 13. 1.4 Metal and Insulator in Solids 13 the two-center approximation as tiνjν = ϕ∗ iν(r − Ri)v(r − Ri)ϕiν (r − Rj )dr. (1.50) Note that we have taken into account in HCoulomb only the intra-atomic Coulomb interactions and omitted the inter-site Coulomb interaction contributions for sim- plicity. It is not easy to treat the electrons in solids described by the Hamiltonian (1.47) because both the electron hoppings and the Coulomb repulsions have to be taken into consideration. In order to discuss both the itinerant and localized behaviors of electrons in solids, we can consider a simpler Hamiltonian consisting of one orbital per site as follows. H = iσ ε0niσ + ijσ tij a† iσ ajσ + i Uni↑ni↓. (1.51) Here ε0, tij , and U denote the atomic level, the transfer integral between sites i and j, and the intra-atomic Coulomb interaction energy, respectively. The Hamilto- nian (1.51) is known as the Hubbard model, and was proposed by Gutzwiller and Hubbard independently [6–10]. The Hubbard model (1.51) is the simplest Hamiltonian which describes the motion of interacting electrons in solids. Nevertheless it describes the localiza- tion of electrons as well as their itinerant behavior in solids. Let us consider the atomic limit of the model. For an atom, we have 4 atomic states: the empty state (n↑ = 0,n↓ = 0), the single electron states (n↑ = 1,n↓ = 0) and (n↑ = 0,n↓ = 1), and the doubly occupied state (n↑ = 1,n↓ = 1). Associated energies are given as 0, ε0, ε0, and 2ε0 + U, respectively. An unﬁlled shell with spin S = 1/2 appears only for the n = 1 state. Note that there is no Hund’s rule arrangement for spin in this case. In the atomic limit for a solid where tij = 0, electron number ni on each atom is no longer constant, though the total number of electrons N is given; N = iσ niσ . The eigenstates are given by |Ψ = |{niσ } , i.e., a set of the electron numbers with spin σ on site i. The eigenenergy for the state is given by E {niσ } = i (ε0ni + Uni↑ni↓). (1.52) It should be noted that the energy of the system increases by U when the number of doubly occupied states D is increased by one. The ground-state energy E0 of the atomic limit is obtained by minimizing the energy with respect to the number of double occupancy in solid. Assume that the number of lattice points is given by L. When N < L, the ground-state energy is obtained as E0 = ε0N by choosing D = 0. Magnetic moments on the sites with an electron are active in this case as shown in Fig. 1.3. Because there are L!/N!(L − N)! electron conﬁgurations on the L lattice points, the ground state is [2N L!/N!(L − N)!]-fold degenerate.
14. 14. 14 1 Introduction to Magnetism Fig. 1.3 Electron conﬁgurations for less than half ﬁlling (upper ﬁgure) and for more than half ﬁlling (lower ﬁgure) in the atomic limit At half ﬁlling, all the atoms are occupied by an electron so that spin de- grees of freedom by 2N remain; the degenerated wave functions are given by |1s1z1s2z1s3z ... when the wave function |{niσ } is written as |n1s1zn2s2zn3s3z ... by using the charge ni = ni↑ + ni↓ and the spin siz = (ni↑ − ni↓)/2. When the electron number N is larger than L, it is no longer possible to keep D = 0; the minimum value of D is given by D = N −L. The ground state energy is then given by E0 = ε0N +U(N −L). The ground state is [22L−N L!/(2L−N)!(N − L)!]-fold degenerate because there are L!/(2L − N)!(N − L)! conﬁgurations for choosing 2L − N(< L) sites with the single electron from L lattice sites and there are 22L−N spin degrees of freedom for each conﬁguration. Note that the spins on 2L − N sites are active in this case. Let us consider the case that electron hopping tij is small but ﬁnite. When N = L, electrons are mobile at T = 0 because electrons can move from site to site without increasing the double occupation number D. Thus the system is a metal. However, at half-ﬁlling, electron hopping creates a doubly occupied state, thus creating a ﬁnite excitation energy by the amount of Coulomb interaction energy U. Therefore elec- trons cannot move under the inﬁnitesimal electric ﬁeld. We have then an insulator with local magnetic moments at each site in this case. When there is no Coulomb interaction (U = 0), on the other hand, electrons are generally itinerant. The Hamiltonian is given as H = ijσ (H0)ij a† iσ ajσ . (1.53) Here (H0)ij = ε0δij + tij (1 − δij ). The noninteracting Hamiltonian is diagonalized by a unitary transformation aiσ = k akσ i|k (a† iσ = k a† kσ i|k ∗) so that H = kσ εknkσ , (1.54) where εk = ij k|i (H0)ij j|k is an eigen value for the tight-binding one-electron Hamiltonian matrix H0, and the set { j|k } (j = 1,...,L) is the eigen vector for εk.
15. 15. 1.4 Metal and Insulator in Solids 15 The eigen states for noninteracting Hamiltonian H are given by |Ψ = |{nkσ } , i.e., a set of electrons with momentum k and spin σ. The eigenenergy is given by E {nkσ } = kσ εknkσ , (1.55) where the c-number nkσ takes on the value of 0 or 1. The ground state is obtained by putting electrons on the energy levels from the bottom to the Fermi level εF according to the Pauli principle, |φ0 = εk<εF kσ a† kσ |0 , (1.56) so that the ground-state energy is given by E0 {nkσ } = εk<εF kσ εk. (1.57) Alternatively, deﬁning the density of states per atom per spin as ρ(ε) = 1 L k δ(ε − εk), (1.58) we can express the ground-state energy per atom as E0 = 2 εF −∞ ερ(ε)dε. (1.59) A non-interacting electron system is in general metallic unless the electrons in the atom form a closed shell. The electrons in such systems are mobile. This is because one can add an electron at the energy level just above the Fermi level by applying inﬁnitesimal electric ﬁeld. Note that spins of itinerant electrons are also mobile. We may expect that there is a transition from metal to insulator at half ﬁlling when the intra-atomic Coulomb interaction is increased. Assume that there is a band for a non-interacting system whose band width is W. The center of the gravity of the noninteracting band is assumed to be located at ε0. When the Coulomb interaction U is increased, each atom tends to be occupied by one electron, and electron hopping to neighboring sites tends to be suppressed in order to reduce the on-site Coulomb interaction energy. In the strongly correlated region, an electron should have a potential ε0 + U on a site having an opposite-spin electron because of the increment of the Coulomb interaction energy due to double occupation, while an electron has a potential ε0 on an empty site. We then expect one more band with the band width of order of W around ε0 + U. The density of states as excitation spectrum is expected to split into two bands at Uc ∼ W (see Fig. 1.4). The formation
16. 16. 16 1 Introduction to Magnetism Fig. 1.4 The upper and lower Hubbard bands created by on-site Coulomb interaction U Fig. 1.5 NaCl type structure in NiO of a gap at the Fermi level implies the existence of an insulator. The insulating state therefore may be realized by the electron correlations when U > W. (1.60) This is Hubbard’s alloy analogy picture to the metal–insulator transition [9, 10]. The metal–insulator transition due to electron correlations as mentioned above is commonly known as the Mott transition. The split bands are named the upper and lower Hubbard bands, respectively. The insulator caused by the electron correlations is referred as the Mott insulator. The concept of the Mott insulator was ﬁrst proposed by Mott [11]. He consid- ered the case of NiO. NiO has the NaCl structure in which Ni–O chain network is formed along [100] direction (see Fig. 1.5). The electronic conﬁguration of the Ni28 (O8) atom is given by 1s22s22p63s23p63d84s2 (1s22s22p4). The oxygen atoms are considered to form a closed shell in the compound taking electrons from Ni atoms, so that we have Ni2+ : 1s2 2s2 2p6 3s2 3p6 3d8 O2− : 1s2 2s2 2p6 . In this case, the Fermi level should be on the d bands in the crystalline system, and we can expect a metal because the 5-fold d bands overlap each other in general (see Fig. 1.6).
17. 17. 1.4 Metal and Insulator in Solids 17 Fig. 1.6 Density of states for NiO in the paramagnetic state obtained by the band calculation [12]. The vertical dashed line shows the Fermi level Experimental results however indicate that NiO is an insulator. To clarify the insulating behavior, Mott considered the electron hopping on the NiO network. Let us estimate an excitation energy Eg when an electron moves to the neighboring Ni2+ site. This process is similar to an excitation of the H2 molecule to a polarized state. Ni2+ O2− 2 −→ Ni3+ O2− + Ni+ O2− . Assume that the intra-atomic Coulomb interaction is given by i (νσ,ν σ ) U · niνσ niν σ for simplicity. There an electron is coupled to the remaining 7 electrons via the on-site Coulomb interaction. After the hopping, the electron is coupled to 8 electrons at the neighboring site, so that the Coulomb interaction is increased by U. On the other hand, the kinetic energy gain due to electron hopping at Ni3+ and Ni2+ sites may be given by 2z|t| ∼ W, (1.61) because electrons in surrounding Ni sites can enter into the Ni3+ ions and the elec- trons in Ni2+ ions can jump to the surrounding Ni sites. Here z is the number of Ni nearest neighbors, and t is an effective electron hopping between Ni atoms. Note that |t| corresponds to an energy gain for the formation of the bonding state due to electron hopping in the H2 molecule, while U corresponds to the Coulomb energy loss in the polarized state. The excitation energy of an electron hopping is therefore given by Eg ∼ U − W. (1.62) Thus, we again have the same criterion for the formation of the Mott insulator (1.60) from the condition Eg > 0. The magnetic materials in the insulator are considered to be the Mott-type insu- lator in which the atomic magnetic moments are built up in the unﬁlled shell. CrO2 and CrBr2 are typical ferromagnetic insulators, while MnO, FeO, CoO, and NiO
18. 18. 18 1 Introduction to Magnetism are known as antiferromagnetic insulators in which the atomic magnetic moments change their direction alternatively from site to site. On the other hand, there are many magnetic metals where the polarized electrons are mobile. These materials are referred as the metallic magnets or itinerant electron magnets. The magnetic properties of these systems are known as the metallic mag- netism or itinerant magnetism. Fe, Co, and Ni are typical examples of the metallic ferromagnet, while Cr and Mn alloys show the antiferromagnetism. We describe in this book the itinerant magnetism of metals and alloys. 1.5 Quenching of Orbital Magnetic Moments The expectation value of the total orbital magnetic moment ML = L is usu- ally quenched in the crystalline system due to the crystalline potential of electrons. Let us consider the case where the spin–orbit interactions are negligible as in the 3d transition metals, and that the magnetic ﬁeld is not applied. Moreover we may assume in solids that the ground state is nondegenerate. One can then choose the ground-state wave function to be real; Ψ ∗ = Ψ . The angular momentum L is real because it is a physical quantity: L = L ∗ . (1.63) Using the relation Ψ ∗ = Ψ , the r.h.s. of the above equation is written as L ∗ = − Ψ |L|Ψ . (1.64) Therefore (1.63) indicates that L = 0. (1.65) Thus, one can expect in metals with sufﬁciently small spin–orbit interactions that only spin magnetic moments contribute to the magnetization. M = 2S . (1.66) This is referred as the quenching of orbital magnetic moments. In the atomic system, electrons are bound by the nuclei, and the orbital angular momentum is ﬁnite in general according to Hund’s second rule. In the crystalline system, the Coulomb energy gain leading to Hund’s second rule is not expected be- cause electrons can hop to the neighboring sites to reduce the Coulomb energy, and electrons can move turning around to right and left (see Fig. 1.7). It may lead to L = 0. This is a physical reason for the quenching of orbital moments in solids. In the 3d transition metals and alloys which we will discuss, the orbital magnetic mo- ments are usually quenched. In the system with a large spin–orbit coupling such as the rare-earth metals or the system with a strong magnetic ﬁeld, the orbital moments remain.
19. 19. 1.6 Heisenberg Model 19 Fig. 1.7 Concept of orbital magnetic moments in atom (L = 0: left) and solids (L = 0: right) 1.6 Heisenberg Model In the insulator, magnetic behaviors are often described by a simple Hamiltonian known as the Heisenberg model. We brieﬂy discuss the Hamiltonian and related properties of the insulator magnetism in this section. Let us consider the hydrogen molecule. We assume one orbital for each hydrogen atom, ϕ1 for atom 1 and ϕ2 for atom 2, and neglect the overlap integrals for simplic- ity, i.e., ϕ1|ϕ2 = 0. The Hamiltonian for the hydrogen molecule is obtained from (1.13) as we derived (1.47). H = iσ ε0niσ + ijσ tij a† iσ ajσ + i Uni↑ni↓ + K − 1 2 J n1n2 − 2Js1 · s2. (1.67) Here K and J denote the intersite Coulomb and exchange integrals given by K = dr dr ϕ∗ 1 (r)ϕ∗ 2 (r )ϕ2(r )ϕ1(r) |r − r | , (1.68) J = dr dr ϕ∗ 1 (r)ϕ∗ 2 (r )ϕ1(r )ϕ2(r) |r − r | . (1.69) In the atomic subspace where n1 = n2 = 1 and the electron hopping is sup- pressed, the Hamiltonian (1.67) reduces as follows. H = 2ε0 + K − 1 2 J − 2Js1 · s2. (1.70) It is diagonalized with the use of the total spin S (in the representation of S and Sz) as H = 2ε0 + K − J S(S + 1) − 1 . (1.71) Therefore the hydrogen molecule has the energy 2ε0 + K − J for the triplet state and 2ε0 + K + J for the singlet state when the inter-site atomic distance is large. This is the Heitler–London theory for the hydrogen molecule. The last term in (1.70) denotes an interaction between the atomic spins s1 and s2. In general, the following Hamiltonian showing the interactions between atomic
20. 20. 20 1 Introduction to Magnetism spins {Si} is known as the Heisenberg model. H = − (i,j) Jij S1 · S2. (1.72) The interaction Jij = 2J in the Heitler–London theory is the inter-site exchange integral due to the Coulomb interaction. This coupling in the Heisenberg model is referred as the direct exchange interaction. The direct exchange interaction is generally positive in sign (i.e., ferromagnetic). Another type of the Heisenberg model with effective exchange coupling is pos- sible in the insulator. In order to derive the effective Hamiltonian, we ﬁrst derive the perturbative effective Hamiltonian from a more general point of view [13]. The effective Hamiltonian is constructed such that it yields the same energy eigen values in a subspace as in the original Hamiltonian acting on the full Hilbert space. Let us consider a subspace P spanned by a set of states {|s }, and introduce a projection operator P = s |s s| which projects any state onto subspace P. The projection operator which chooses the complementary subspace Q is deﬁned by Q = 1 − P . Note that P2 = P , Q2 = Q, and PQ = QP = 0. The eigen value problem of the original Hamiltonian H is written as (H − E)ψ = 0. (1.73) Inserting the identity 1 = P + Q into the above equation as (P + Q)(H − E)(P + Q)ψ = 0 and multiplying P from the l.h.s. of the equation, we obtain (PHP − E)P + PHQ ψ = 0. (1.74) In the same way, we can derive the following equation QHP + (QHQ − E)Q ψ = 0. (1.75) In (1.74) and (1.75), the wave function ψ is separated into two components be- longing to different subspaces, Pψ and Qψ. From both equations, one can elim- inate the wave function Qψ that leads to the eigenvalue equation in subspace P, namely, PHP − PHQ(QHQ − E)−1 QHP Pψ = EPψ. (1.76) The above equation indicates that the following Hamiltonian Hp(E) acting on the wave function Pψ in the subspace P is regarded as an effective Hamiltonian which yields the same eigen value E as in the original Hamiltonian H, where Hp(E) = PHP − PHQ(QHQ − E)−1 QHP. (1.77) The effective Hamiltonian depends on the energy which should be obtained self- consistently. Taking the subspace spanned by a subset of the eigenfunctions of an
21. 21. 1.6 Heisenberg Model 21 unperturbed Hamiltonian, one can derive the effective Hamiltonian which is cor- rect up to the second order of the interaction Hamiltonian. Assume that the Hamil- tonian consists of a noninteracting part H0 and an interaction part HI such that H = H0 +HI. The eigenvalues {E0 k } and eigenfunctions {φk} for H0 are assumed to be known. We deﬁne the subspace P spanned by a part of {|φk }. The projection op- erator is then deﬁned by P = P μ |φμ φμ|. We have the relation QHP = QHIP , and thus obtain the effective Hamiltonian which is correct up to the second order in interaction, after having replaced the Hamiltonian H and the energy E in the denominator of (1.77) with the zeroth-order ones, H0 and E0 k , i.e., Hp = PHP − PHIQ QH0Q − E0 k −1 QHIP. (1.78) The effective Hamiltonian depends on the eigen state k explicitly. Therefore we rewrite the second term as follows. QH0Q − E0 k −1 QHIPφk = P μ Q ν E0 ν − E0 μ −1 |φν φν|HI|φμ φμ|φk . (1.79) Thus the perturbative Hamiltonian (1.78) is expressed as follows. Hp = PHP − PHIQ E0 Q − E0 P −1 QHIP. (1.80) Here E0 P (E0 Q) denotes the eigenvalues belonging to subspace P (Q). The eigen value equation for the perturbative effective Hamiltonian is then given by HpPψk = EkPψk. (1.81) We can derive the effective Heisenberg model in the strong Coulomb interac- tion regime at half-ﬁlling using the formula (1.80). Let us consider the Hubbard model (1.51). As found in Sect. 1.4, the ground state of the atomic limit at half- ﬁlling is speciﬁed by {ni = 1} states. The ground state is 2L-fold degenerate, L being the number of sites. We start from the ground state in the atomic limit at half ﬁlling, i.e., the {ni = 1} states, and deﬁne the subspace P from them. The complementary subspace Q consists of the subspace containing empty states and the subspace containing the doubly occupied states. In the strongly correlated re- gion, the electron hopping rate |tij | is much smaller than the Coulomb interac- tion strength U, so that the Hamiltonian H is separated into the atomic state H0 = iσ ε0niσ + i Uni↑ni↓ and the ‘interaction’ term HI = ijσ tij a† iσ ajσ . The ﬁrst term at the r.h.s. of (1.80) is given by PLε0P . In the calculations of the second term, we have QHIP = ijσ tij a† iσ ajσ P because a† iσ ajσ P belong to the space Q. Moreover, E0 Q − E0 P = U when it is operated on the single doubly- occupied state QHIP . Thus we obtain the expression for the second term at the r.h.s.
22. 22. 22 1 Introduction to Magnetism of (1.80) as follows. PHIQ E0 Q − E0 P −1 QHIP = ijklσσ tlktij U Pa† lσ akσ a† iσ ajσ P. (1.82) Among the summation at the r.h.s. of (1.82) only the k = i and l = j terms remain. Rearranging the creation and annihilation operators, we obtain the relation. σσ a† jσ aiσ a† iσ ajσ = nj − 1 2 ninj − 2si · sj . (1.83) Substituting the above relation into (1.82), we obtain the following effective Hamil- tonian. Hp = P L ε0 − 1 2 j |tij |2 U + (i,j) 4|tij |2 U si · sj P. (1.84) Apart from the constant term, we arrive at the following effective Heisenberg model in the strong Coulomb interaction regime at half ﬁlling, which operates on the sub- space P. H = − (i,j) Jij s1 · s2. (1.85) Here Jij = − 4|tij |2 U . (1.86) The effective exchange integral (1.86) is known as the super exchange interaction because it is caused by a virtual exchange of electrons belonging to different atoms via transfer integrals. The super exchange interaction is antiferromagnetic, while the direct exchange interaction (1.69) is ferromagnetic. Note that the subspace on which the Hamiltonian (1.85) acts is given by {P|n1s1z,n2s2z,... } = {|1s1z,1s2z,... }. This can be simpliﬁed as {|s1z,s2z,... }. In many magnetic insulators, anions are often located between the magnetic ions. In such a case, the super exchange interac- tion becomes dominant. The Heisenberg model (1.85) is not justiﬁed in the metallic system where the band width W ∼ U. Nevertheless, we often ﬁnd the same type of the intersite magnetic interactions, which are useful for qualitative understanding of the magnetism (see Sects. 6.4 and 8.3 for examples). 1.7 Magnetic Structure Magnetic materials have their microscopic structure for arrangement of atomic mag- netic moments. This is called the magnetic structure. The structure characterizes the
23. 23. 1.7 Magnetic Structure 23 magnetic property as well as the electronic structure. In this section, we introduce the Fourier representation of the magnetic structure and explain brieﬂy the magnetic structures in solids. The magnetic structure is characterized by the magnetic moment density which is given by M(r) = ψ† (r)mψ(r) . (1.87) Here ψ(r) = (ψ↑(r),ψ↓(r)) is the ﬁeld operator of electrons. m denotes the mag- netic moment for an electron as given by (1.7). In a crystalline system, we may divide the space into the Wigner–Seitz cells for each atom. Then we can deﬁne a magnetic moment of atom i as follows. mi = i M(r)d3 x. (1.88) Here the integration is over the Wigner–Seitz cell belonging to atom i. In a non- crystalline system we may adopt the Voronoi polyhedra instead of the Wigner–Seitz cells. In the case of the crystalline system, the atomic position Rl is expressed by using the primitive translational vectors a,b,c as Rl = l1a + l2b + l3c. (1.89) The atomic magnetic moment is expanded with use of the Fourier lattice series as follows. ml = q m(q)eiq·Rl . (1.90) Here q is the wave vector in the ﬁrst Brillouin zone. The Fourier components of the magnetic moments are given as m(q) = 1 L l mle−iq·Rl , (1.91) L being the number of lattice points. Note that m(−q) = m(q)∗ because ml are real. Moreover we assumed that there is only one atom per unit cell. When there are more than one atom per unit cell, we have to add the atomic position in a unit cell ηλ to (1.89). Accordingly, the magnetic moments (1.90) and (1.91) are speciﬁed by the type of atom λ as m (λ) l (m(λ)(q)). Hereafter we consider the crystalline system with one magnetic atom per unit cell. The microscopic magnetic structure of magnetic materials is speciﬁed by a set of {ml} or {m(q)}. The simplest structure is that all of the atomic magnetic moments have the same direction. It is realized when all the Fourier components vanish except m(q = 0) = m, and is known as the ferromagnetic structure (see Fig. 1.8). Typical transition metals such as Fe, Co, and Ni exhibit the ferromagnetism.
24. 24. 24 1 Introduction to Magnetism Fig. 1.8 Ferromagnetic arrangement Fig. 1.9 Antiferromagnetic arrangement The antiferromagnetic structure (AF) is deﬁned by alternative arrangement of the atomic magnetic moments along a direction, e.g., the z direction (see Fig. 1.9). It is speciﬁed by a set, m(±Q) = mk exp(±iα) and m(q = ±Q) = 0, where Q consists of half a reciprocal lattice vectors, and k denotes a unit vector along the z axis, and α denotes a phase of the structure. In the case α = 0, we have ml = mk cos(Q · Rl). (1.92) When the position Rl moves along Q vector, Q · Rl changes by π. Accordingly, the magnetic moment ml changes its sign. The AF structure on the simple cubic lattice as shown in Fig. 1.10(a) is expressed by the wave vector Q = (K1 + K2 + K3)/2 = (1,1,1)π/a, a being the lattice con- stant. The AF structure on the body-centered cubic lattice as shown in Fig. 1.10(b) is expressed by the wave vector Q = (−K1 + K2 + K3)/2 = (0,0,1)2π/a. In the case of the face-centered cubic lattice (fcc) structure, two kinds of AF structures are known. The AF structure of the ﬁrst-kind as shown in Fig. 1.10(c) is described by a wave vector Q = (K2 + K3)/2 = (0,0,1)2π/a. The atomic moment alternatively changes the direction with a translation by (0,0,1)a/2. It is also possible to change direction alternatively along 1 1 1 axis. This is referred as the AF structure of the second-kind, and is characterized by Q = (K1 + K2 + K3)/2 = (1,1,1)π/a (see Fig. 1.11). Cr with 1 at% Mn on the bcc lattice shows the AF structure, and γ -Mn on the fcc lattice shows the AF structure of the ﬁrst-kind according to the neutron diffraction experiments. It should be noted that the network consisting of the up-spin atoms (or the down- spin atoms) forms a lattice referred as the sublattice. There are two sublattices in the antiferromagnetic structures shown in Fig. 1.10. Each sublattice forms the fcc lattice with the lattice constant 2a in the case of the sc structure (Fig. 1.10(a)), the sc lattice with the lattice constant a in the case of the bcc structure (Fig. 1.10(b)), and the simple tetragonal structure with the lattice constants a/ √ 2 and a in the case of the fcc structure (Fig. 1.10(c)), respectively. The sinusoidal spin density wave (SDW) structure is expressed by ml = mk sin(Q · Rl + α), (1.93) where Q vector is neither equal to 0 nor to the AF wave vectors. The magnetic moment sinusoidally changes with a period λ = 2π/|Q| along the Q direction (see
25. 25. 1.7 Magnetic Structure 25 Fig. 1.10 Antiferromagnetic arrangements on the simple cubic lattice (a), body-centered cubic lattice (b), and face-centered cubic lattice (c). The lattice constants are shown by a Fig. 1.11 The antiferromagnetic structure of the second-kind on the face-centered cubic lattice Fig. 1.12 Spin density wave structure Fig. 1.12). Note that the period is not necessarily commensurate with the lattice spacing in general. Cr is a well-known example of the SDW. It is also possible that the magnetic moment rotates with a translation (see Fig. 1.13). This is known as the helical structure, and is expressed as ml = m e1 cos(Q · Rl + α) + e2 sin(Q · Rl + α) . (1.94) Here e1 and e2 are the unit vectors being orthogonal to each other. The magnetic moment with amplitude m rotates on the e1–e2 plane with the translation along the Q vector. The above expression (1.94) can also be written as ml = m(Q)eiQ·Rl + m(Q)∗ e−iQ·Rl , (1.95) with m(Q) = m 2 (e1 − ie2)eiα . (1.96) It indicates that the helical structure is speciﬁed by the Q vector and the condition m(Q)2 = 0. (1.97)
26. 26. 26 1 Introduction to Magnetism Fig. 1.13 Helical structure (left) and conical structure (right) Fig. 1.14 2Q multiple- spin-density wave structure It is known from the neutron experiments that Au2Mn, MnO2, CrO2, Eu, Tb, Dy, Ho etc. show the helical structure. So far the magnetic structures are characterized by only one Q vector. One can also consider the helical type structure with the bulk magnetization as follows. ml = mzk + m i cos(Q · Rl + α) + j sin(Q · Rl + α) . (1.98) The above expression is alternatively written as ml = mzk + m(Q)eiQ·Rl + m(Q)∗ e−iQ·Rl , (1.99) with m(Q)2 = 0. (1.100) This is referred as the conical magnetic structure (see Fig. 1.13). The magnetic mo- ment rotates for example on the x–y plane when the moment translates along the direction of Q.
27. 27. 1.7 Magnetic Structure 27 Fig. 1.15 3Q multiple- spin-density wave structure One can also consider a magnetic structure consisting of two wave vectors, Q1 and Q2. For example, we can consider a structure such as ml = m(Q1)eiQ1·Rl + m(Q2)eiQ2·Rl + c.c. (1.101) Assuming that m(Q1) = mxi/2 and m(Q2) = mxj/2, we have ml = mxi cos(Q1 · Rl) + myj cos(Q2 · Rl). (1.102) This is known as a double Q multiple SDW (2Q-MSDW) (see Fig. 1.14). In the case of the fcc lattice, we may consider the wave vectors Q1 = (1,0,0)2π/a and Q2 = (0,1,0)2π/a. Then the x(y) component changes the sign with a translation Rl = (1,0,0)a/2 (R2 = (0,1,0)a/2) as shown in Fig. 1.14. We can also consider the magnetic structure consisting of three wave vectors Q1, Q2 and Q3, which is the so-called triple Q multiple SDW (3Q-MSDW). For example, we have a 3Q-MSDW such that ml = mxi cos(Q1 · Rl) + myj cos(Q2 · Rl) + mzk cos(Q3 · Rl), (1.103) with Q1 = (1,0,0)2π/a, Q2 = (0,1,0)2π/a, and Q3 = (0,0,1)2π/a. Each com- ponent changes sign after the translation by a/2 along the same direction as shown in Fig. 1.15. In the substitutional disordered alloys, we have more complicated structures which cannot be described by a small number of wave vectors. When we take a conﬁgurational average of the atomic magnetic moments, we can deﬁne the aver- age magnetization [ml]c. Here [∼]c denotes the conﬁgurational average. In some Fig. 1.16 Spin glass arrangement
28. 28. 28 1 Introduction to Magnetism cases, an ordered state with randomly oriented magnetic moments referred as the spin glass (SG) appears (see Fig. 1.16). The SG is considered to be characterized by the condition such that [ml]c = 0 and m2 l c = 0. (1.104) The disordered dilute alloys such as Cu1−xMnx (x 0.1) and Au1−xFex (x 0.1) are known to show a SG at low temperatures (see Sect. 7.1). Experimentally most magnetic structures of crystalline systems are determined by the neutron elastic scattering experiments. The readers who are interested in the experimental determination of the magnetic structure are recommended to refer to the books by Marshall and Lovesey [14, 15].
29. 29. http://www.springer.com/978-3-642-33400-9